1.
IOSR Journal of Pharmacy Vol. 2, Issue 3, May-June, 2012, PP.579-592 PROCESS OPTIMIZATION AND BIOSORPTION OF LEAD USING ALBIZIA SAMAN LEAF POWDER Rao, P.J1, Kumari, R.S1,Babji J.S2, Naga Lakshmi, N.V.R3 and Raju, Ch.A.I.1* 1 Department of Chemical Engineering, Andhra University, Visakhapatnam – 530 003 2 Department of Computer Science and Systems Engineering, Andhra University, Visakhapatnam – 530 003 3 Department of Petroleum Engineering, GIET College of Engineering, RajahmundryABSTRACTWater pollution is one of the signs that humans have exceeded the limits and causing health problems for living beings onearth. The present paper comprises the optimization and biosorption of lead from aqueous solution using Albizia saman leafpowder as biosorbent. Single Step Optimization was considered for preliminary runs with the variables agitation time,biosorbent size, pH of the solution, initial concentration of the aqueous solution, dosage of biosorbent and temperature. TheCentral Composite Design (CCD) was used for final runs optimization using Response Surface Methodology (RSM). Resultsindicated that the optimum agitation time for biosorption of lead is 50 min. The increase in mass of biosorbent lead toincrease in lead (pb) ion biosorption due to the increase in the number of active biosorption sites. Maximum percentagebiosorption is observed at a pH of 6 and with particle size of 53 µm. Experimental data were better described by pseudo-second-order model. The adsorption isotherm could be well fitted by the Langmuir equation followed by Freundlich andTemkin. Over and all, Albizia Saman leaf powder can be used as an effective natural biosorbent for the economic treatmentof aqueous solutions containing lead.Keywords - Albizia Saman, biosorption, optimization, isotherms, kinetics1. INTRODUCTION Because of its relative recent development in the planets history, pollution is a human problem. Before the 19thcentury Industrial Revolution, people lived more in harmony with their immediate environment. If one or more substanceshave built up in resources like water, air etc., to such an extent that they cause problems for living beings, we treat it aspolluted one. As industrialization has spread around the globe, the problem of pollution spread along with it. Intensivemining operations and processing of minerals to meet the increasing needs of our society have led to environmental pollutionin specific locations all over the world [1]. Heavy metals are discharged from various industries such as electroplating, plasticmanufacturing, textile, storage batteries, mining and metallurgical process [2]. Water pollution of toxic heavy metal ionsdischarged from the industries and inhabited areas is seriously harmful to the health of human beings and the eco-system.Among these heavy metals, lead may be the severe pollutant sources due to its wide applications in industries, which mayproduce wastewater containing lead at the concentrations higher than the recommended doses of 0.015 mg/L.Microorganisms immobilized on natural and synthetic adsorbents have been used for separation and preconcentration ofheavy metals at trace levels [3, 4, 5, 6, 7]. Most studies have focused on the removal of Pb2+, Cd2+, and Ni2+ from wastewaterby using various biosorbents [8]. Biosorbents are prepared from the naturally abundant or waste biomass of algae, moss,fungi or bacteria [9]. Hence the naturally and abundantly available albizia saman has been selected for the present study forthe removal of lead from aqueous solutions.2. MATERIALS AND METHODS2.1 Biosorbent Preparation Albizia saman leaves were obtained from Rajahmundry. The leaves are washed thrice with tap water and once withdistilled water in order to remove adhering mud, impurities etc. It was dried in sunlight for one week until all the moisturewas evaporated. The crispy powder were then crushed and grinded to powder, separated using British Standard Sieves (BSS)and stored in dry vacuum packs to prevent moisture content and readily used as biosorbent.2.2 Batch sorption studies Preliminary experiments were conducted in 250 ml Erlenmayer flasks containing 50 ml of 20 mg/L metal solutionusing single step optimization procedure. The flasks were agitated on an orbital shaker at 180 rpm and samples were taken atpredetermined time intervals (1, 3, 5, 10, 15, 20, 25, 30, 40, 50, 60, 90, 120, 150 & 180 min) & centrifuged at 14000 rpm andthe supernatant liquid was analysed in Atomic Absorption Spectrophotometer (AAS) for final concentrations. Similarly theother variables were varied in a wide range: Biosorbent Size (53, 75, 104, 125 & 152 µm), pH of the aqueous solution (2, 3,4, 5, 6, 7 and 8), Initial concentration of lead solution (25, 30, 60, 120 & 180 mg/L), Biosorbent Dosage (10, 20, 30, 40, 50 &60 g/L) and Temperature (283, 293, 303, 313 & 323 K).2.3 Process optimization ISSN: 2250-3013 www.iosrphr.org 579 | P a g e
2.
IOSR Journal of PharmacyVol. 2, Issue 3, May-June, 2012, PP.579-592 Final experimental runs for optimization were obtained through Response Surface Methodology from Design ofExperiments (DoE) using STATISTICA software. The extent of biosorption of lead calculated at the preliminary optimumconditions is verified with the final runs for the optimum conditions.3. RESULTS AND DISCUSSION The potential of dry Albizia saman leaf powder as a biosorbent for the biosorption of lead metal present in anaqueous solution is investigated in the present investigation. The effects of various parameters on biosorption of lead arestudied. The numerical analysis of the investigation was undertaken applying CCD using RSM.3.1 Effect of agitation time The equilibrium agitation time is determined by plotting the % biosorption of lead against agitation time as shown infig. 1. For 0.5g (10 mg/L) of biosorbent and 53μm of biosorbent size in the interaction time intervals of 1 to180 min 58.30 %(1.166 mg/g) of lead is biosorbed in the first 1 min. The % biosorptionis increased briskly up to 50 min reaching 79.45 %(1.589 mg/g). Beyond 50 min, the % biosorption is constant indicating the attainment of equilibrium conditions. Themaximum biosorption of 79.45% (1.589 mg/g ) is attained for 50 min of agitation time with 10 g/L of 53 μm size biosorbentmixed in 50 mL of aqueous solution (C0=20 mg/L) [10, 11].3.2 Effect of biosorbent size The percentage biosorption is increased from 72.12 (1.4424 mg/g) to 79.45 % (1.589 mg/g) as the biosorbent sizedecreases from 152 to 53 μm presented in fig. 2. This phenomenon is expected, as the size of the particle decreases, surfacearea of the biosorbent increases; thereby the numbers of active sites on the biosorbent are better exposed to the biosorbate.3.3 Effect of pH of the aqueous solution In order to determine the optimal value, pH of the aqueous solution is varied from 2 to 8. The pH of aqueoussolution is shown against % biosorption of lead in fig 3. The % biosorption of metal is increased from 58.42 % (1.1684 mg/g)to 77.18 % (1.5436 mg/g) as pH is increased from 2 to 6 and decreased beyond pH value of 7. The predominant sorbingforms of lead are Pb2+ and PbOH+ that occurr in the pH range of 4–6. This is the reason for higher biosorption of lead in thepH range of 4–6. At pH higher than 6, precipitation of lead occurred and biosorption due to biosorption is reduced [12, 13,14].3.4 Effect of initial concentration of lead in the aqueous solution The effect of initial Pb2+ ion concentration is investigated in the range of 20-180 mg/L. The effect of initialconcentration of lead in the aqueous solution on the percentage biosorption of lead is shown in fig. 4. The percentagebiosorption of lead is decreased from 77.12% to 58.68% with an increase in C0 from 20 mg/L to 180 mg/L while the uptakecapacity is increased from 1.5424 to 10.5624 mg/g [15]. 3.5 Effect of biosorbent dosage The biosorption of lead increases from 77.14% (1.5428 mg/g) to 83.78 % (0.5585 mg/g) with an increase inbiosorbent dosage from 10 to 30 g/L, shown in fig. 5. Such behavior is obvious because with an increase in biosorbentdosage, the number of active sites available for lead biosorption would be more. The change in percentage biosorption of leadis marginal from 83.78% (0.5585 mg/g) to 84.92% (0.2830 mg/g) when ‘w’ is increased from 30 to 60 g/L. Hence all otherexperiments are conducted at 30 g/L dosage.3.6 Effect of temperature The effect of temperature on the equilibrium metal uptake was significant. The effect of changes in the temperatureon the lead uptake is shown in fig. 6. When temperature was lower than 303 K, Lead uptake increased with increasingtemperature, but when temperature was over 303 K, the results slowed down and the increase is marginal. This responsesuggested a different interaction between the ligands on the cell wall and the metal. Below 303 K, chemical biosorptionmechanisms played a dominant role in the whole biosorption process, biosorption was expected to increase by increase in thetemperature. While at higher temperature, the plant powder was in a nonliving state, and physical biosorption became themain process. Physical biosorption reactions were normally exothermic, thus the extent of biosorption generally is constantwith further increasing temperature [16]. ISSN: 2250-3013 www.iosrphr.org 580 | P a g e
3.
IOSR Journal of PharmacyVol. 2, Issue 3, May-June, 2012, PP.579-5923.7 Isotherms3.7.1 Langmuir isotherm Irving Langmuir developed an isotherm named as Langmuir isotherm, which is the most widely used simple two-parameter equation. Langmuir isotherm is drawn between Ce vs Ce/ qe shown in fig 7. The equation obtained is (Ce/qe) =2.8729 Ce + 0.05929 with a good linearity (correlation coefficient, R2=0.9791) indicating strong binding of lead ions to thesurface of albizia saman leaf powder. The separation factor (RL) of 0.9219 shows favorable biosorption (0< RL<1). Hence amaximum biosorption capacity of the Albizia saman leaf powder for lead is find to be 16.8656 mg/g by Langmuir isothermsat 303K (mass of biosorbent: 10 g/L) [17, 18].3.7.2 Freundlich isotherm Freundlich empirical adsorption isotherm equation can be applied in case of low and intermediate concentrationranges. Freundlich isotherm is drawn between log qe and log Ce, in fig. 8 The equation obtained is log qe = 0.6815 log Ce –0.2404. The resulting equation has a correlation coefficient of 0.9655. The ‘n’ value in the above equations is 0.6815,satisfies the condition of 0<n<1 indicating favorable biosorption. Kf is 0.5748 mg/g [19].3.7.3 Temkin isotherm Temkin and Pyzhev isotherm equation describes the behavior of many adsorption systems on the heterogeneoussurface. The present data are analysed according to the linear form of Temkin isotherm and the linear plot is shown in fig. 9The equation obtained for lead biosorption is: q e = 3.1546 ln Ce -3.8813 with a correlation coefficient 0.9637. The best fitmodel is determined based on the linear regression correlation coefficient (R2) [20].3.8 Kinetics of biosorption Kinetic models are used to describe the order of biosorbate – biosorbent interactions. Traditionally, the first ordermodel of Lagergren finds wide application. In the case of biosorption preceded by diffusion through a boundary, the kineticsin most cases follows the first order rate equation of Lagergren [21]:(dqt/dt) = K1 (qe – qt)where qe and qt are the amounts adsorbed at t, min and equilibrium time and Kad is the rate constant of the first orderadsorption.The above equation can be presented aslog (qe – qt) = log qe – (K1/2.303) tlog (qe – qt) = –0.02357 t – 0.3027 ; R2 = 0.9620Plot of log (qe–qt) versus ‘t’ gives a straight line for first order kinetics, facilitating the computation of biosorption rateconstant (K1). If the experimental results do not follow the above equation, they differ in two important aspects:K1 (qe – qt) does not represent the number of available adsorption sites and log q e is not equal to the intercept.In such cases, pseudo second order kinetic equation [22, 23]:(dqt/dt ) = K2 (qe – qt)2 is applicable, where ‘K2’ is the second order rate constant.The other form of the above equation is:(t/qt) = (1/ K2qe2) + (1/qe) t(t/qt) = 0.6229 t + 1.1720; R2 = 0.9959The pseudo second order model based on above equation, considers the rate-limiting step as the formation of chemisorptivebond involving sharing or exchange of electrons between the biosorbate and biosorbent. If the pseudo second order kinetics isapplicable, the plot of (t/qt) versus ‘t’ gives a linear relationship that allows computation of q e and K2.In the present study, the kinetics are investigated with 50 mL of aqueous solution (C 0= 20 mg/L) at 303 K with the interactiontime intervals of 1 min to 50 min. Lagergren and pseudo plots for biosorption of lead with biosorbent size 53 μm of Albiziasaman leaf powder are drawn in figs. 10 & 11. As the correlation coefficient values for the pseudo second order kinetics is0.99 which is better than first order kinetics (R2=0.962), very well describes the biosorption mechanism of lead using Albiziasaman leaf powder.3.9 Thermodynamics of biosorption The process of Biosorption is temperature dependant. In general, the temperature dependence is associated withthree thermodynamic parameters namely change in enthalpy of biosorption (∆H), change in entropy of biosorption (∆S) andchange in Gibbs free energy (∆G).The Van’t Hoff’s plots for the biosorption data obtained at initial concentrations of the lead are shown in fig. 12. Theequation obtained is log qe / Ce = –0.41701(1/T) + 0.5921. The correlation coefficient is 0.9568. In the present study, theenthalpy change is ∆H is 7.9845 J/mole is positive indicating that the biosorption is endothermic. The value of ∆S is 11.3370J/mole is also positive indicating the irreversibility of process, ∆G is 3427.1334 J/mole is negative indicating the spontaneityof biosorption. ISSN: 2250-3013 www.iosrphr.org 581 | P a g e
4.
IOSR Journal of PharmacyVol. 2, Issue 3, May-June, 2012, PP.579-5923.10 Optimization of the selected parameters using CCD In order to determine an optimum condition for lead ions removal, the parameters having greater influence over theresponse are to be identified. In the present study, the relationship between four independent variables and percent of leadions biosorption is fitted well with the quadratic model. The regression equation for the optimization of lead biosorption: %biosorption of lead (Y) is a function of the W (X1), Co (X2), pH (X3), and T (X4). Table–1 presents the coded levels and Table–2 represents the variations in the corresponding coded values of four parameters and response based on experimental runs andpredicted values proposed by CCD design.Y = –452.007 + 0.429 X1 + 0.369 X2 + 5.846 X3 + 3.347 X4 – 0.006X12 – 0.015X22 – 0.548 X32 – 0.006 X42 + 0.004 X1X2 –0.010 X1X3 + 0.026 X2X3 + 0.002 X3X4 -------------------------------- (1)Interpretation of the regression analysis: The results of above regression model for Eq. (1) (in the form of analysis of variance ANOVA) are compiled inTable-3. In general, the Fischer’s ‘F-statistics’ value (=MSmodel/MSerror), where MS (mean square) with a low probability ‘P’value indicates high significance of the regression model. The ANOVA of the regression model demonstrates that the modelis highly significant, as is evident from the Fisher’s F-test (Fmodel = 33852) and a very low probability value (Pmodel >F=0.000000). More over, the computed F-value (F0.05 (14.15) = MSmodel/MSerror = 33852) is greater than that of the tabular F-value (F0.05 (14.15) tabulars = 2.42) at the 5% level, indicating that the treatment differences are significant.The significance of the regression coefficient of the parameter can be verified by the Student’s t-test as a tool, while ‘P’values signify the pattern of interaction among the factors. From the Table–4, we can observe that, the larger the value of tand smaller the value of P, more significant is the corresponding coefficient term. By analyzing the ‘t’ values and ‘P’ valuesfrom Table-4, it is found that the X1, X2, X3, X4, X12 , X22 , X32 , X42 X1X2, X1X3, X1X4, X2X3, X2X4, X3X4 have high significanceto explain the individual and interaction effect of biosorption variables on the biosorption of lead to predict the response. A positive sign of the coefficient represents a synergistic effect which means response (% biosorption of leadincreases with the increase in effect, while a negative sign indicates an antagonistic effect which means response (%biosorption of lead) decreases with the increase in effect. The optimal set of conditions for maximum percentage biosorptionof lead is pH = 6.0250, biosorption dosage (w) = 31.7191 g/L, initial lead concentration (C o) = 19.8996 mg/L andtemperature = 304.0673 K. The extent of biosorption of lead calculated at these optimum conditions is 84.90612%. Fig. 13shows the comparison between the % biosorption obtained through experiments and predicted. The correlation coefficient(R2) provides a measure of the models variability in the observed response values. The closer the R2 value to 1, the strongerthe model is and it predicts the response better. In the present study the value of the regression coefficient (R 2 = 0.99997)indicates that 0.003% of the total variations are not satisfactorily explained by the model. The ANOVA Table-3 can be usedto test the statistical significance of the ratio of mean square due to regression and mean square due to residual error.Figs. 15 to 20 were represented as a function of two factors at a time, holding other factors fixed at zero level for theInteraction effects of biosorption variables. ISSN: 2250-3013 www.iosrphr.org 582 | P a g e
5.
IOSR Journal of PharmacyVol. 2, Issue 3, May-June, 2012, PP.579-5924. FIGURES AND TABLES 85 biosorbent=albizia saman leaf power 80 %biosorption of lead 75 Dp=53m w=10g/L T=303K 70 C0=20mg/L pH=6.8 65 % biosorption of lead 60 55 0 20 40 60 80 100 120 140 160 180 200 agitation time, t min Fig. 1 Effect of agitation time on % biosorption of lead 90 1.60 88 Biosorbent = Albizia saman leaf power 1.58 86 1.56 W=10g/L T= 303K % biosorption of lead 84 pH= 6.8 1.54 t =50min metal uptake 82 C0=20mg/L 1.52 80 1.50 78 1.48 76 1.46 74 % biosorption 72 metal uptake 1.44 70 1.42 40 60 80 100 120 140 160 Biosorbent size m Fig. 2 Variations in % biosorption of lead using biosorbent sizes 80 2.0 Biosorbent= Albizia saman leaf power 75 1.8 % biosorption % biosorption of lead metal uptake metal uptake 70 1.6 65 1.4 Dp=53m T=303K W=10 g/L t = 50min 60 1.2 C0=20 mg/L 55 1.0 1 2 3 4 5 6 7 8 9 pH of aqueous solution Fig. 3 Effect of pH on % biosorption of lead ISSN: 2250-3013 www.iosrphr.org 583 | P a g e
6.
IOSR Journal of PharmacyVol. 2, Issue 3, May-June, 2012, PP.579-592 80 12 Biosorbent= Albizia saman leaf power 10 75 % biosorption metal uptake % biosorption of lead 8 metal uptake 70 6 65 4 Dp=53m T=303K 60 pH= 6 2 W=10g/L t =50min 55 0 0 20 40 60 80 100 120 140 160 180 200 initial concentration of aqueous solution, mg/L Fig. 4 Effect of initial concentration for the biosorption of lead 86 1.8 Biosorbent =Albizia saman leaf power 1.6 84 1.4 % biosorption % Biosorption of lead metal uptake 1.2 Metal uptake 82 Dp=53m 1.0 T=303K 80 pH=6 C0=20mg/L 0.8 t=50min 0.6 78 0.4 76 0.2 0.0 0.5 1.0 1.5 2.0 2.5 3.0 3.5 Biosorbent dosage, W, g/L Fig. 5 Effect of biosorbent dosage on % biosorption of lead 86 Biosorbent = Albizia saman leaf powder 85 0.58 % biosorption 84 metal uptake % biosorption of lead 0.56 83 metal uptake 82 Dp=53m pH=6 0.54 C0=20 mg/L 81 W=30 g/L t=50min 80 0.52 79 78 0.50 280 290 300 310 320 330 Temperature, K Fig. 6 Effect of temperature for the biosorption of leadISSN: 2250-3013 www.iosrphr.org 584 | P a g e
7.
IOSR Journal of PharmacyVol. 2, Issue 3, May-June, 2012, PP.579-592 8 Biosorbent = Albizia saman leaf power 7 91 .97 2 =0 6 ,r 92 92 .05 Ce/qe gm/L +0 C e 29 5 .87 =2 /q e Dp= 53 m C e W = 10 g/L 4 T =303 K pH =6.0 t = 50min 3 2 0 10 20 30 40 50 60 70 80 Ce Fig. 7 Langmuir isotherm for biosorption of lead 1.2 Biosorbent = Albizia saman leaf power 1.0 55 .96 0.8 2 =0 ,r 04 24 -0. Ce log qe log 0.6 15 .68 =0 Dp= 53 m q e log W = 10 g/L 0.4 T =303 K pH =6.0 t = 50min 0.2 0.0 0.4 0.6 0.8 1.0 1.2 1.4 1.6 1.8 2.0 log Ce Fig. 8 Freundlich isotherm for biosorption of lead -2 Biosorbent = Albizia saman leaf power 0 q e =3 .15 46 2 lnC e- -3 .88 13 ,r2 Dp= 53 m =0 .96 qe 4 37 W = 10 g/L T =303 K pH =6.0 t = 50min 6 8 10 1.0 1.5 2.0 2.5 3.0 3.5 4.0 4.5 ln Ce Fig. 9 Temkin isotherm for biosorption of leadISSN: 2250-3013 www.iosrphr.org 585 | P a g e
8.
IOSR Journal of PharmacyVol. 2, Issue 3, May-June, 2012, PP.579-592 -1.4 Biosorbent = Albizia saman leaf power -1.2 20 .96 2 =0 ,r 27 -1.0 .30 7 t-0 35 02 -0. )= log (qe-qt) -0.8 -q t (q e log Dp= 53 m -0.6 W = 10 g/L T =303 K pH =6.0 -0.4 C0=20 mg/L -0.2 0.0 0 10 20 30 40 50 t, min Fig. 10 First order kinetics for biosorption of lead 35 Biosorbent = Albizia saman leaf power 30 25 59 2 0. 99 20 r= 0, 72 t+1.1 t/qt 15 9 Dp= 53 m 22 =0.6 W = 10 g/L t/q t T =303 K 10 pH =6.0 C0=20 mg/L 5 0 0 10 20 30 40 50 60 t, min Fig. 11 Second order Kinetics for biosorption of lead -0.65 Biosorbent = Albizia saman leaf power -0.70 log q/ e C e =-0 -0.75 .41 70 (1 / t) +0 logqe/Ce .59 21 -0.80 , r2 Dp= 53 m =0.9 56 W = 10 g/L 8 t =50 min -0.85 pH =6.0 C0=20 mg/L0=20 mg/L -0.90 -0.95 3.0 3.1 3.2 3.3 3.4 3.5 3.6 1/t x 103min Fig. 12 Vant Hoff’s plot for biosorption of leadISSN: 2250-3013 www.iosrphr.org 586 | P a g e
9.
IOSR Journal of PharmacyVol. 2, Issue 3, May-June, 2012, PP.579-592 Fig. 13 Predicted vs Observed Fig. 14 Pareto Chart Fig. 15 Surface contour plot for the effects of dosage and initial concentration of lead on % biosorptionISSN: 2250-3013 www.iosrphr.org 587 | P a g e
10.
IOSR Journal of PharmacyVol. 2, Issue 3, May-June, 2012, PP.579-592 Fig. 16 Surface contour plot for the effects of dosage and pH on % biosorption of lead Fig. 17 Surface contour plot for the effects of dosage & Temperature on % biosorption of lead Fig. 18 Surface contour plot for the effects of initial concentration and pH on % biosorption of leadISSN: 2250-3013 www.iosrphr.org 588 | P a g e
11.
IOSR Journal of PharmacyVol. 2, Issue 3, May-June, 2012, PP.579-592 Fig. 19 Surface contour plot for the effects of initial concentration and Temperature on % biosorption of lead Fig. 20 Surface contour plot for the effects of pH and Temperature on % biosorption of lead TABLE–1 Levels of different process variables in coded and un-coded form for % biosorption of lead using Albizia saman leaf powder Var Name Range and levels -2 -1 0 1 2 X1 Biosorbent dosage, 10 20 30 40 50 w, g/L X2 Initial concentration, 10 15 20 25 30 Co, mg/L X3 pH of aqueous 4 5 6 7 8 solution X4 Temperature, T, K 283 293 303 313 323ISSN: 2250-3013 www.iosrphr.org 589 | P a g e
13.
IOSR Journal of PharmacyVol. 2, Issue 3, May-June, 2012, PP.579-592 Table–4 Estimated regression coefficients for the lead biosorption onto Albizia saman leaf powder Terms Regression Standard error of t-value P-value coefficient the coefficient Mean/Intercept -452.007 1.335753 -338.391 0.000000 Dosage, w, g/L (L) 0.429 0.005629 76.293 0.000000 Dosage, w, g/L (Q) -0.006 0.000014 -439.689 0.000000 Conc, Co, mg/L (L) 0.369 0.011310 32.663 0.000000 Conc, Co, mg/L (Q) -0.015 0.000055 -273.032 0.000000 pH (L) 5.846 0.057298 102.035 0.000000 pH (Q) -0.548 0.001365 -401.230 0.000000 Temperature, T, K (L) 3.347 0.008391 398.867 0.000000 Temperature, T, K (Q) -0.006 0.000014 -403.061 0.000000 1L by 2L 0.004 0.000036 120.992 0.000000 1L by 3L -0.010 0.000179 -58.048 0.000000 1L by 4L -0.000 0.000018 -13.288 0.000000 2L by 3L 0.026 0.000357 72.036 0.000000 2L by 4L -0.000 0.000036 -6.294 0.000014 3L by 4L 0.002 0.000179 10.491 0.0000005. CONCLUSION Both Preliminary and finals experimental runs are carried out to find out the equilibrium, isotherms, kinetics andthermodynamic parameters for biosorption of lead from an aqueous solution using Albizia saman leaf powder. The analysisof the experimental and theoretical data results in the conclusions that the equilibrium agitation time for lead biosorption is50 minutes. The % biosorption of lead from an aqueous solution increased from 72.12 to 79.45 % with a decrease in theparticle size of the biosorbent from 152 to 53 µm and increases from 77.14 to 83.78 % with increase in biosorbent dosagefrom 10 to 30 g/L. With an increase in the initial concentration of lead in the aqueous solution (20 to 180 mg/L), thepercentage biosorption of lead from the aqueous solution is decreased from 77.12 to 58.68 %. Percentage biosorption of leadfrom the aqueous solution increased significantly with increase in pH from 2 to 6 (58.42 to 77.18 %). Hereafter, percentagebiosorption decreases for further increase in pH from 6 to 8 (77.18 to 69.42 %). The maximum uptake capacity of 16.8656mg/g is obtained at a temperature of 303 K. The present study involves the use of statistical experimental design to optimizeprocess conditions for maximal biosorption of lead from aqueous solution using CCD involving RSM. The maximumbiosorption of lead (84.90612 %) onto Albizia saman leaf powder is observed when the processing parameters are set asfollows: pH = 6.0250, w = 31.7191 g/L, Co = 19.8996 mg/L and T = 304.0673 K. The kinetic studies showed that thebiosorption of lead is better described by pseudo second order kinetics. The thermodynamic data depicted that % biosorptionof lead increased with increase in temperature up to some extent. ISSN: 2250-3013 www.iosrphr.org 591 | P a g e
14.
IOSR Journal of PharmacyVol. 2, Issue 3, May-June, 2012, PP.579-592REFERENCES [1] Prerna Ahuja, Rani Gupta, R.K. Saxena, Sorption and Desorption of Cobalt by Oscillatoria anguistissima, Current Microbiology Vol. 39, 1999, pp. 49–52 [2] Ahmet Çabuk, Tamer Akar, Sibel Tunali, Özge Tabak, Biosorption characteristics of Bacillus sp. ATS-2 immobilized in silica gel for removal of Pb(II), Journal of Hazardous Materials, Volume 136, Issue 2, 21, 2005, Pages 317–323 [3] Volesky, B., Removal and recovery of heavy metals by biosorption [C] Volesky B, ed. Biosorption of Heavy Metals (Boca Raton: CRC Press, 1990) 12–13. [4] Volesky, B, Biosorption of Heavy Metals (CRC Press, Boca Raton 1990). [5] Lo, W., Chua, H., Lam, K.H., Bi, S.P., A comparative in`vestigation on the biosorption of lead by filamentous fungal biomass, Chemosphere 39, 1999, 2723–2736. [6] Alaa H. Hawari, Catherine N. Mulligan, Biosorption of lead(II), cadmium(II), copper(II) and nickel(II) by anaerobic granular biomass, Bioresource Technology 97, 2006, 692–700. [7] Ankit Balaria, Silke Schiewer, Assessment of biosorption mechanism for Pb binding by citrus pectin, Separation and Purification Technology 63, 2008, 577–581. [8] Anushree Malik, Metal bioremediation through growing cells, Environment International 30, 2004, 261– 278. [9] Arzu,Y.and Dursun,A., Comparative study on determination of the equilibrium, kinetic and thermodynamic parameters of biosorption of copper (II) and lead (II) ions onto pretreated Aspergillus niger, Biochem.Eng. J., 28, 2006, 187-195. [10] Chandrasekhar K, Subramanian S, Modak JM, Natarajan KA, Removal of metals using an industrial biomass with reference to environmental control, Int J Miner Process 53, 1998, 107–120. [11] K. Parvathi, R. Nareshkumar R. Nagendran, Biosorption of lead by Aspergillus niger and Saccharomyces cerevisiae, World J Microbiol Biotechnol 23, 2007, 671–676. [12] R.N. Sylva, The environmental chemistry of copper (II) in aquatic systems, Water Res. 10, 1976, 789–792. [13] O. Masala, E.J.L. McInnes, P. Obrien, Modelling the formation of granules: the influence of lead ions on calcium pyrophosphate precipitates, Inorg, Chim. Acta 339, 2002, 366–372. [14] Goyal N, Jain SC, Banerjee, Comparative studies on the microbial adsorption of heavy metals, Adv Environ Res 7, 2003, 311–319. [15] Sag, Y., D. Ozer and T. Kutsal, A comparative study of the biosorption of lead(II) ions to Z. ramigera and R. arrhizus, Process Biochem., 30, (2), 1995, 169-174. [16] R.H.S.F. Vieira, B. Volesky, Biosorption: a solution to pollution, Int. Microbiol. 3, 2000, 17–24. [17] I. Langmuir, The constitution and fundamental properties of solids and liquids. Part 1: Solids, J. Am. Chem. Soc., 38, 1916, 2221–2295. [18] I. Langmuir, The adsorption of gases on plane surface of glass, mica and platinum, J. Am. Chem. Soc., 40, 1918, 1361–1403. [19] H. Freundlich, Uber die adsorption in losungen (Adsorption in solution), Z. Phys. Chemie., 57, 1906, 384- 470. [20] M.J Temkin and V Pyzhey, Recent modifications to Langmuir isotherms, Acta Physiochim., 12, 1940, 217– 222. [21] S. Lagergren, On the theory of so called adsorption of dissolved substances, Handlingar, 24, 1898, 1–39. [22] Y.S. Ho and G McKay, A Comparison of Chemisorption Kinetic Models Applied to Pollutant Removal on Various Sorbents, Process Safety and Environmental Protection, 6B, 1998, 332-340. [23] Y.S. Ho and G. McKay, Pseudo-second order model for sorption processes, Process Biochemistry, 34, 1999, 451–465.ISSN: 2250-3013 www.iosrphr.org 592 | P a g e
Views
Actions
Embeds 0
Report content